## Plaquette Valence Bond Theory of Cuprate

## High-Temperature

## Superconductivity

### Malte

### Harland

1,*_{,}

_{Tim}

_{Berberich}

1_{,}

_{Mikhail}

_{I.}

_{Katsnelson}

2_{,}

_{Alexander}

_{I.}

_{Lichtenstein}

1,3
1_{Institute}_{of}_{Theoretical}_{Physics,}_{University}_{of}_{Hamburg,}_{Hamburg,}_{20355,}_{Germany}

2_{Institute}_{for}_{Molecules}_{and}_{Materials,}_{Radboud}_{University,}_{Nijmegen,}_{6525AJ,}_{the}_{Netherlands}

3_{The}_{Hamburg}_{Centre}_{for}_{Ultrafast}_{Imaging,}_{Hamburg,}_{22761,}_{Germany}

Copyright©2018 by authors, all rights reserved. Authors agree that this article remains permanently open access under the terms of the Creative Commons Attribution License 4.0 International License

### Abstract

We investigate the phenomenon of high-temperature superconductivity within a strong coupling perspective. The occurence is traced to a quantum critical point that is in the phase diagram of the plaquette’s t,t0-Hubbard model. We develop a bottom-up approach combining several methods, i.e. exact diagonalizationof an isolated plaquette, the Lanczos-method for a plaquette within a bath and cluster dynamical Mean-Field theory with continuous time quantum Monte-Carlo solver to embedd the plaquette in a lattice environment. The quantum criticalpointis locatedwheretheN =2,3,4-sectorsof the plaquette cross. This point is also found to show optimal doping. The dx2_{−}y2 -wave order turns out to be largest at the localized-itinerant transition of the electrons. Furthermore, we present an explenation for the pseudo-gap phenomenon, that is explained by a soft mode related to local singlets of the plaquette.The theory presented here is similar to the resonating valence bond theory, but stresses the importance oflocalsinglets.

### Keywords

Quantum Critical Point, Plaquette, Hubbard Model, Resonating Valence Bonds### 1

### Introduction

After 30 years history of extremely intensive experi-mental [1–4] and theoretical [5–10] studies of the high-temperature superconductivity (HTSC) in copper oxides we are still far from understanding the basic mechanism of this fascinating phenomenon. Taking into account the enormous number of researchers involved in this field, one can assume that almost all possible ideas were ex-pressed and that the main problem is just to select the basic simple concepts from the pile of available theo-retical results. The most ambitious attempt was made by P. W. Anderson who emphasized with his resonat-ing valence bond (RVB) theory the crucial importance of strong electron correlations, the tendency to singlet

spin state formation and the non-Fermi liquid
charac-ter of the normal phase [6]. Unfortunately, details of
his original approach, such as suppression of interlayer
hopping in the normal phase as the main factor of
super-conductivity, seems to contradict experimental data [11].
The latest version of the RVB theory is presented in [12].
We believe, that the main assumption of the strongly
correlated limit as the base of understanding the
high-temperature superconductivity is correct, as well as
em-phasizing a crucial role of spin singlet states, but
impor-tant details were missing. Below we present arguments
for the thesis, that the minimal object of HTSC-theory
is the plaquette in the so-called effective t, t0 Hubbard
model [13], rather than the conventional atomic limit
typical for the theory of Mott insulators [6, 9]. The best
practical realization of this atomic based theory is the
dynamical mean-field theory (DMFT) [14]. The
obvi-ous minimal generalization in the case of dx2_{−}_{y}2-wave

pairing is a cluster DMFT (CDMFT) scheme [15, 16].

Since the first plaquette CDMFT calculation of
dx2_{−}_{y}2-wave superconducting order together with

anti-ferromagnetic fluctuations [15], there have been many
calculations for different cluster sizes and
geome-tries based on continuous-time Quantum Monte Carlo
(CTQMC) or exact diagonalization (ED) solvers [17–
23, 16, 24–31]. Unfortunately, the basic qualitative
fea-ture of the many-body states in the plaquette were
hid-den in computational details. The main aim of this work
is to present a simple and transparent strong coupling
theory of the dx2_{−}_{y}2-wave superconductivity, i.e. a

min-imalconsistent many-body model, based on the plaque-tte energy spectrum peculiarity, namely the “quantum critical point”, that merges two singlets and two dou-blets. These states of the doped plaquette are different from those discussed in the resonating valence-bond the-ory [6, 12]. The main point is that the quantum critical point discussed here is related to the formation of lo-calvalence bonds in thefrustratedquantum spin model [32]. Therefore, the optimal superconducting states are located on the border between localized and delocalized resonating plaquette valence bonds. Here we follow a bottom-up approach starting with an isolated plaquette

Universal Journal of Physics and Application 12(4): 76-81, 2018 http://www.hrpub.org

and building stepwise a more complex environment. An important theoretical problem is to find a minimal and generic electronic-structure model of cuprate super-conductors. From band structure calculations [13] we can safely reduce it to an effective one-band model with long-range hopping. We use a standard parametrization of the tight-binding model for YBa2Cu3O7[13] with the

next-nearest neighbor hopping: t0/t=−0.3 andtas unit of our energies. The local Hubbard interaction parame-ter U is of the order of the bandwidth W = 8t. Then, thet, t0 Hubbard model on the square lattice reads

H =−X

ij

tijc†iσcjσ+

X

i

U ni↑ni↓, (1)

where tij is an effective hopping and U the local
Coulomb interaction. The operatorsc†_{iσ}, ciσ create and
annihilate fermions at site iwith spin σ=↑(+),↓(−),
respectively and the occupation operator isniσ=c†_{iσ}ciσ.

### 2

### Isolated Plaquette

We start the discussion with electronic states in the isolated Hubbard plaquette. The optimal doping for high-temperature superconductivity is of the order of 15% of holes per site for almost all cuprate materials. This gives us an average number of electrons per site of 0.85 and results in 3.4 fermions per 4-site plaquette in the crystal. We argue, that this is related to 3-electron states of the isolated plaquette, since particle-hole asym-metry introduced by the next-nearest neighbor hopping t0, with moderate values ofU and certain fixed chemical potentials (µ) result in an occupation per plaquette of the crystal, that is very close to the optimal value of 3.4 electrons.

The Hamiltonian of the isolated plaquette reads

Hp= X

(i,j)=1..4

h0_{ij}c†_{iσ}cjσ+ X
i=1..4

U ni↑ni↓, (2)

−ˆh0=

µ t t0 t t µ t t0 t0 t µ t t t0 t µ

.

We include the chemical potential in the diagonal part ofh0

ij. We present in Fig. 1 regions in theU −µspace, whose ground states have an occupation of three plus-minus one electrons. The one-electron spectrum pos-sesses four states with the energies: ±2t−t0−µ and double-degenerate t0 −µ. At zero interaction U = 0, there is no stable ground state with three electrons, in the sense that one can add or remove one electron with-out changing the thermodynamic potential. Starting from some critical interaction strength U ≈ 3 there is a small region, in that the plaquette ground state with N = 3 electrons is separated by energy gaps from the states withN = 2 andN = 4, see Fig. 1. Importantly, this N = 3 ground state is fourfold degenerate consist-ing of two doublets in the sectors (2↑,1↓) and (1↑,2↓), which we label|Xiand|Yi, according to their symme-try. Moreover, there is a critical point (circle in Fig. 1) where all three sectors with 2, 3, and 4 electrons have the same ground state energy and form a sixfold degen-erate ground-state multiplet consisting of two singlets of

the sectors (1↑,1↓) and (2↑,2↓) together with two
dou-blets of the 3-electron sectors. This critical point has
the coordinates U = 2.78, µ = 0.24 for the standard
value of t0/t = −0.3. At smaller t0 this critical point
shifts to larger U and at t0/t = 0 its coordinates are
U = 4.58, µ = 0.72. We think, that this critical point
of the plaquette has crucial importance for the physics
of the strong-coupling dx2_{−}_{y}2-wave superconductivity.

Here, we demonstrate via bottom-up approach, that this is the key ingredient of a consistent minimal picture of HTSC.

2 3 4 5 6 7 8

U

0.0 0.2 0.4 0.6 0.8 1.0

µ

N

2 3 4

Figure 1. Zero-temperature phase diagram of the isolated
pla-quette as function of HubbardUand chemical potentialµin
prox-imity of the quantum critical point (circle) fort0_{/t}_{=}_{−}_{0.3.}

If we approach this critical point from the region with the N = 3 ground state, then the one electron density of states (DOS) at the Fermi energy diverges for both, electron and hole sides, due to transitions from the four-fold degenerateN= 3 ground state to singlets ofN = 2 (hole side) and N = 4 (electron side) with zero excita-tion energy. The corresponding spectral weights with normalization of the δ-functions are equal to 0.46 and 0.23 for hole and electron sides, respectively. Thus, it introduces an important electron-hole asymmetry.

In Fig. 2 we show static observables of the plaquette in very close proximity to the critical point. The local charge is denoted by circles and the nearest-neighbor Heisenberg-spin correlations by strips. Shown are all six states of the different particle number sectors. Dark (light) circles denote electrons (holes) occupying the re-spective site and dark (light) strips triplet (singlet)-like correlations. Regarding this set of observables, the N = 2 and the N = 4 states obey the Z4-symmetry.

But the spin-doublets of N = 3 reduce it toZ2, which

is exactly the d-wave symmetry. Due to the rotation symmetry, we can relate the orbitals of the plaquette to high-symmetry points of the lattice’s Brillouin zone, i.e. G, X, Y and M. Although d-wave pairing takes place in the antinodal X and Y directions, we learn from the doublets in Fig. 2, that correlations of the nodal direction M are involved, which agrees with re-cent experimental results.[33, 34] The Z2 symmetry of

the N = 3 states changes to Z4 at U = 6.18(dashed

is understood for largeU by e.g. mapping to thet−J -model[17]. A calculation of a plaquette observable with exact-diagonalization does always weighten the degen-erate N = 3 states equally and their superposition pre-seves the plaquette’s symmetry. However, a coupling to another system has potetntial for creating modes that resonate stronger with one of the doublet states than with the others.

0.45 0.45

1.54 1.54 0.45 0.45

1.0 1.0

1.0 1.0

0.72 0.71

0.41 1.34 0.71 0.72

0.61 0.89

0.89 0.61

0.71 0.72

1.34 0.41 0.72 0.71

0.89 0.61

0.61 0.89

1.03 0.4

1.0 0.75 0.4 1.03

0.79 0.71

0.71 0.79

0.4 1.03

0.75 1.0 1.03 0.4

0.71 0.79

0.79 0.71

0.49 0.49

0.39 0.39 0.49 0.49

0.5 0.5

0.5 0.5

Figure 2. Static observables of the local charge (circles) and the nearest-neighbor Heisenberg-spin correlations(strips) in proximity of the critical point for N = 2 (top left), N = 4 (bottom left) and the four-fold degenerateN = 3 (mid, right). In case of the doublets the total spin along quantization axis is indicated by a black arrow.

### 3

### Plaquette in Bath

The appearance of the DOS peak at the Fermi
en-ergy leads to a universal instability in the sense, that
the susceptibility diverges in many different channels
(magnetic, superconducting, charge density wave, etc.).
In order to study the interplay of different instability
channels from the strong-coupling perspective we
intro-duce a simple model of an embedded plaquette in the
spirit of DMET [35]. To this aim we add to the
plaque-tte’s Hamiltonian a hybridization with four fermionic
bath states, one bath state per corner of the plaquette.
We use an exact diagonalization technique, namely the
Lanczos scheme with a Hilbert space size of 216_{, without}

any symmetry restrictions. Furthermore, we introduce
different symmetry breaking fields acting on the bath
fermions b†_{iσ}, bjσ, i.e. dx2_{−}_{y}2-wave pairing, singlet

mag-netic states on the bonds, and the conventional N´eel antiferromagnetic state:

hd= X

σ=↑,↓,i=1..4

(−1)iσ∆d(bi,σbi+1,−σ+h.c.), (3)

hs=

X

σ=↑,↓,i=1..4

(−1)iσ∆s(b†i,σbi+1,−σ+h.c.), (4)

hm=1 2

X

σ=↑,↓,i=1..4

(−1)iσ∆mb†_{i,σ}bi,σ. (5)

Here we assume periodic boundary conditions, that
means for i = 4 we define i+ 1 = 1. We switch on
small fields ∆d = ∆s = ∆m = 0.01t simultaneously
and calculate numerically their associated
susceptibili-ties of the plaquette. The hybridization V between the
fermionsc†_{iσ}andb†_{jσ} breaks the sixfold degeneracy of the

plaquette’s quantum critical point and without external
fields it results in a singlet ground state. The dx2_{−}_{y}2

-wave superconducting 3 and the magnetic bond-singlet 4 external fields respect quantum entanglement of the singlet character of the ground state, whereas the N´eel field 5 destroys it. Being classical in its nature, the N´eel state is expected to be most stable for sufficiently strong coupling with the environment V [36] or high tempera-tures [37].

0.0 0.2 0.4 0.6 0

2 4

s

m

d

S

u

s

c

e

p

t

i

b

i

l

i

t

y

V/t

Figure 3. Superconducting (χd), singlet bond order (χs) and

antiferromagnetic (χm) susceptibility of the plaquette in a bath

as a function of the hybridizationV forU= 3 andµ= 0.27.

For an infinite system different types of order can be
found by studying divergences of susceptibilities. Since
in DMET we deal with finite systems, the
susceptibili-ties remain finite up to zero temperature and we assume,
that the largest susceptibility of the cluster signals the
corresponding order of the crystal. The computational
results are shown in Fig. 3 as function of the
hybridiza-tion parameter V. One can see, that dx2_{−}_{y}2-wave

su-perconducting pairing always wins in comparison with
the singlet bond pairing and is more favorable than the
N´eel order forV ≤ 0.2. The self-consistent
plaquette-Bethe DMFT for the cluster case (see below) with
opti-mal HTSC parameters corresponds toV = 0.1. The
sin-glet ground state near the plaquette’s quantum critical
point favors dx2_{−}_{y}2-wave superconductivity, rather than

magnetic ordering. This result agrees well with large scale CDMFT calculations for optimal doping [27, 28].

There are three main contributions by the single-plaquette sectors with N = 2,3,4 electrons, which have almost equal spectral weights. In particular, it means a strong mixture of states, that differ by two electrons, i.e. by a local Cooper pair on the bond. This is understood as an important detail for superconductivity, since the degenerate quantum critical point (circle in Fig. 1) con-sists of states with the same total number of electrons (Ntot= 8), but none of those shows a double occupation on the plaquette. It occurs only on bath sites, that have no Hubbard interaction. The degeneracy of the quan-tum critical point splits into four states forN= 2, eight states for N = 3 and two states forN = 4. Taking into account the total number of these states and including all their antisymmetric singlet combinations, we observe, that 85% of the ground state components are related to the quantum critical point. This means, that the system as a whole perfectly screens the strong Coulomb inter-actions (Hubbard U is about 70% of the bandwidth) and the plaquette states withN = 2,3,4 electrons con-tribute equally to the ground state singlet of the total system. A specific symmetry of the ground state at the

plaquette’s quantum critical point increases effectively thesingle-siteU by suppressing double occupations on plaquette sites. But, at the same time, it decreases the effectiveU for the plaquette in a sense, that one does not have to pay an additional energy for adding two more electrons to the plaquette as a whole. This situation is very nontrivial; it demonstrates clearly, that discussions of strong correlations for the high-Tc cuprates would be based on a rather four-orbital Hubbard model, corre-sponding to a lattice built from plaquettes, than on an initial single-band Hubbard model for copper sites.

### 4

### Plaquette CDMFT

Finally, we perform the standard CDMFT calcula-tions using a strong-coupling continuous-time Quantum Monte Carlo solver [38, 39] in the normal state. Since a transition to the periodic plaquette in the crystal in-creases the bandwidth by a factor of two due to doubling of the coordination numbers compared to the isolated plaquette, we increase the values ofU andµby the fac-tor of two. Note, that the natural energy unit is the bandwidthW, rather than the hoppingt. Furthermore, we use the value of U/t = 6, which approximately de-scribes real cuprate materials [40].

The calculated local DOS obtained by maximum-entropy analytic continuation [41] is shown in Fig. (4). We observe, that for sufficiently high temperatures there is a broad peak at the Fermi energy originating from the plaquette quantum critical point. This relation is illus-trated in the inset of Fig. (4). We artificially scaled the hopping between plaquettes by a factor αranging from 0 to the physical value 1.

-4 -2 0 2 4

0.0 0.2 0.4 0.6 0.8 1.0

Figure 4. Density of states for both spins of the plaquette CDMFT forU= 6 andµ= 0.54 for different temperatures.

At lower temperatures a pseudogap is formed. It is well-known in all HTSC materials and considered as one of its most striking features [42]. Sometimes this pseudogap is also considered to be the precursor of the superconducting gap (formation of incoherent Cooper pairs above Tc) or as a smeared antiferromagnetic gap (shadow bands) [42]. However, both interpretations have problems, when they get compared to experiments [42]. Within our scheme it is natural to interpret this pseudogap as a pseudo-hybridization-gap similar to that arising in Kondo lattices [43] or intermediate valence semiconductors [44]. From this point of view the pseudo-gap in HTSC materials originates from the Fano

antires-onance due to embedding of the soft-fermion mode of the plaquette (discussed above) into a continuous band spec-trum of the lattice. The role of soft-fermion modes in a different context, the hidden fermion, has been discussed in [45].

The density of states for optimal doping n = 0.85 in the self-consistent CDMFT calculations is shown in the right inset of Fig. 4. Its chemical potential con-verges to a value of µ = 1.2, which is very similar to that of the fixedµ of the quantum critical point in the isolated plaquette. Furthermore, we have calculated a low-temperature superconducting state with CDMFT, Lanczos solver and 8-bath sites and also with a CTQMC cluster solver and found similar results to many other calculations [17, 19, 20, 23, 16, 24–29].

### 5

### Conclusions

To conclude, we developed a picture of HTSC based on the existence of a quantum critical point at the cross-ing of the ground state energies in theN = 2,3,4 sectors within the plaquette for parameters close to the optimal doping, t0 being of crucial importance. Contrary to the original resonating valence bond (RVB) theory of Ander-son [6], we start with thelocal valence bond formation in the doped plaquette. The optimal superconducting region is related to a localized-delocalized transition of plaquette valence bond states in the plaquette. It would be interesting to describe the formation of global sin-glet states with plaquette valence bond states using the matrix product scheme [46], since the CDMFT scheme breaks translational symmetry.

Formation of the soft-fermion mode near the optimal doping has an analog in the weak coupling theory within the van Hove scenario of HTSC [47, 48]. Due to the for-mation of flat bands of many-body origin [47] there is a whole region of parameterst0, U, µ, in that the Fermi-liquid description is broken. However, we believe that the strong-coupling description presented here is more relevant for real HTSC materials, which are character-ized by large values ofU [40].

### Acknowledgements

A. I. L. acknowledges support from the DFG SFB-668 and The Hamburg Centre for Ultrafast Imaging, M. I. K. acknowledges financial support from ERC (project 338957 FEMTO/NANO) and from NWO via the Spinoza Prize. Computations have been performed at the NIC, Forschungszentrum J¨ulich, under project HHH26.

### REFERENCES

[1] J. G. Bednorz and K. A. M¨uller. Possible hightc su-perconductivity in the balacuo system. Zeitschrift f¨ur Physik B Condensed Matter, 64(2):189–193, 1986.

cuprate superconductors.Rev. Mod. Phys., 75:473– 541, Apr 2003.

[3] J. Orenstein and A. J. Millis. Advances in the physics of high-temperature superconductivity. Sci-ence, 288(5465):468–474, 2000.

[4] M. H. Hamidian, S. D. Edkins, Chung Koo Kim, J. C. Davis, A. P. Mackenzie, H. Eisaki, S. Uchida, M. J. Lawler, E.-A. Kim, S. Sachdev, and K. Fujita. Atomic-scale electronic structure of the cuprate d-symmetry form factor density wave state.Nat Phys, 12(2):150–156, February 2016.

[5] P.W. Anderson. A re-examination of concepts in magnetic metals: The nearly antiferromagnetic fermi liquid.Advances in Physics, 46(1):3–11, 1997.

[6] Philip W Anderson et al. The theory of supercon-ductivity in the high-Tc

cuprate superconductors, volume 446. Princeton University Press Princeton, NJ, 1997.

[7] D. J. Scalapino. A common thread: The pairing in-teraction for unconventional superconductors.Rev. Mod. Phys., 84:1383–1417, Oct 2012.

[8] Jrg Schmalian, David Pines, and Branko Sto-jkovi. Weak pseudogap behavior in the underdoped cuprate superconductors. Journal of Physics and Chemistry of Solids, 59(1012):1764 – 1768, 1998.

[9] Masatoshi Imada, Atsushi Fujimori, and Yoshinori Tokura. Metal-insulator transitions. Rev. Mod. Phys., 70:1039–1263, Oct 1998.

[10] Elbio Dagotto. Correlated electrons in high-temperature superconductors.Rev. Mod. Phys., 66: 763–840, Jul 1994.

[11] H. J. A. Molegraaf, C. Presura, D. van der Marel, P. H. Kes, and M. Li. Superconductivity-induced transfer of in-plane spectral weight in bi2sr2cacu2o8+. Science, 295(5563):2239–2241, 2002.

[12] PHILIP W. ANDERSON. Personal history of my engagement with cuprate superconductivity, 19862010.International Journal of Modern Physics B, 25(01):1–39, 2011.

[13] O.K. Andersen, A.I. Liechtenstein, O. Jepsen, and F. Paulsen. Proceedings of the conference on spectroscopies in novel superconductors lda energy bands, low-energy hamiltonians, t, t, t (k), and j. Journal of Physics and Chemistry of Solids, 56(12): 1573 – 1591, 1995.

[14] Antoine Georges, Gabriel Kotliar, Werner Krauth, and Marcelo J. Rozenberg. Dynamical mean-field theory of strongly correlated fermion systems and the limit of infinite dimensions. Rev. Mod. Phys., 68:13–125, Jan 1996.

[15] A. I. Lichtenstein and M. I. Katsnelson. Antifer-romagnetism and d -wave superconductivity in cuprates: A cluster dynamical mean-field theory. Phys. Rev. B, 62:R9283–R9286, Oct 2000.

[16] Thomas Maier, Mark Jarrell, Thomas Pruschke, and Matthias H. Hettler. Quantum cluster theo-ries. Rev. Mod. Phys., 77:1027–1080, Oct 2005.

[17] Kristjan Haule and Gabriel Kotliar. Strongly cor-related superconductivity: A plaquette dynamical mean-field theory study. Phys. Rev. B, 76:104509, Sep 2007.

[18] M. Ferrero, P. S. Cornaglia, L. De Leo, O. Parcollet, G. Kotliar, and A. Georges. Valence bond dynami-cal mean-field theory of doped mott insulators with nodal/antinodal differentiation. EPL (Europhysics Letters), 85(5):57009, 2009.

[19] Michel Ferrero, Pablo S. Cornaglia, Lorenzo De Leo, Olivier Parcollet, Gabriel Kotliar, and An-toine Georges. Pseudogap opening and formation of fermi arcs as an orbital-selective mott transition in momentum space. Phys. Rev. B, 80:064501, Aug 2009.

[20] Emanuel Gull, Olivier Parcollet, and Andrew J. Millis. Superconductivity and the pseudogap in the two-dimensional hubbard model. Phys. Rev. Lett., 110:216405, May 2013.

[21] E. Khatami, K. Mikelsons, D. Galanakis, A. Macridin, J. Moreno, R. T. Scalettar, and M. Jarrell. Quantum criticality due to incipient phase separation in the two-dimensional hubbard model. Phys. Rev. B, 81:201101, May 2010.

[22] E. Gull, M. Ferrero, O. Parcollet, A. Georges, and A. J. Millis. Momentum-space anisotropy and pseu-dogaps: A comparative cluster dynamical mean-field analysis of the doping-driven metal-insulator transition in the two-dimensional hubbard model. Phys. Rev. B, 82:155101, Oct 2010.

[23] David S´en´echal, P.-L. Lavertu, M.-A. Marois, and A.-M. S. Tremblay. Competition between anti-ferromagnetism and superconductivity in high-Tc cuprates. Phys. Rev. Lett., 94:156404, Apr 2005.

[24] T. A. Maier, M. S. Jarrell, and D. J. Scalapino. Structure of the pairing interaction in the two-dimensional hubbard model. Phys. Rev. Lett., 96: 047005, Feb 2006.

[25] M. Aichhorn, E. Arrigoni, M. Potthoff, and W. Hanke. Phase separation and competition of superconductivity and magnetism in the two-dimensional hubbard model: From strong to weak coupling. Phys. Rev. B, 76:224509, Dec 2007.

[26] E. Gull, P. Werner, X. Wang, M. Troyer, and A. J. Millis. Local order and the gapped phase of the hubbard model: A plaquette dynamical mean-field investigation. EPL (Europhysics Letters), 84(3): 37009, 2008.

[27] M. Civelli. Evolution of the dynamical pairing across the phase diagram of a strongly correlated high-temperature superconductor.Phys. Rev. Lett., 103:136402, Sep 2009.

[28] S. S. Kancharla, B. Kyung, D. S´en´echal, M. Civ-elli, M. Capone, G. Kotliar, and A.-M. S. Tremblay. Anomalous superconductivity and its competition with antiferromagnetism in doped mott insulators. Phys. Rev. B, 77:184516, May 2008.

[29] Satoshi Okamoto and Thomas A. Maier. En-hanced superconductivity in superlattices of high-Tccuprates.Phys. Rev. Lett., 101:156401, Oct 2008.

[30] Xi Chen, J. P. F. LeBlanc, and Emanuel Gull. Su-perconducting fluctuations in the normal state of the two-dimensional hubbard model. Phys. Rev. Lett., 115:116402, Sep 2015.

[31] L Fratino, P Smon, G Sordi, and A-M S Trem-blay. An organizing principle for two-dimensional strongly correlated superconductivity. Scientific Reports, 6:22715–, February 2016.

[32] I Affleck. Exact results on the dimerisation transi-tion in su(n) antiferromagnetic chains. Journal of Physics: Condensed Matter, 2(2):405, 1990.

[33] J. Graf, C. Jozwiak, C. L. Smallwood, H. Eisaki, R. A. Kaindl, D-H. Lee, and A. Lanzara. Nodal quasiparticle meltdown in ultrahigh-resolution pump-probe angle-resolved photoemission. Nat Phys, 7(10):805–809, October 2011.

[34] Christopher L. Smallwood, James P. Hinton, Christopher Jozwiak, Wentao Zhang, Jake D. Ko-ralek, Hiroshi Eisaki, Dung-Hai Lee, Joseph Oren-stein, and Alessandra Lanzara. Tracking cooper pairs in a cuprate superconductor by ultrafast angle-resolved photoemission. Science, 336(6085): 1137–1139, 2012.

[35] Bo-Xiao Zheng and Garnet Kin-Lic Chan. Ground-state phase diagram of the square lattice hubbard model from density matrix embedding theory.Phys. Rev. B, 93:035126, Jan 2016.

[36] H. Hafermann, M. I. Katsnelson, and A. I. Licht-enstein. Metal-insulator transition by suppression of spin fluctuations. EPL (Europhysics Letters), 85 (3):37006, 2009.

[37] Junya Otsuki, Hartmut Hafermann, and Alexan-der I. Lichtenstein. Superconductivity, antifer-romagnetism, and phase separation in the two-dimensional hubbard model: A dual-fermion ap-proach. Phys. Rev. B, 90:235132, Dec 2014.

[38] Emanuel Gull, Andrew J. Millis, Alexander I. Lichtenstein, Alexey N. Rubtsov, Matthias Troyer, and Philipp Werner. Continuous-time monte carlo

methods for quantum impurity models. Rev. Mod. Phys., 83:349–404, May 2011.

[39] Priyanka Seth, Igor Krivenko, Michel Ferrero, and Olivier Parcollet. Triqs/cthyb: A continuous-time quantum monte carlo hybridisation expansion solver for quantum impurity problems. Computer Physics Communications, 200:274 – 284, 2016. [40] B. Dalla Piazza, M. Mourigal, M. Guarise,

H. Berger, T. Schmitt, K. J. Zhou, M. Grioni, and H. M. Rønnow. Unified one-band hubbard model for magnetic and electronic spectra of the parent compounds of cuprate superconductors.Phys. Rev. B, 85:100508, Mar 2012.

[41] Mark Jarrell and J.E. Gubernatis. Bayesian infer-ence and the analytic continuation of imaginary-time quantum monte carlo data. Physics Reports, 269(3):133 – 195, 1996.

[42] Makoto Hashimoto, Inna M. Vishik, Rui-Hua He, Thomas P. Devereaux, and Zhi-Xun Shen. Energy gaps in high-transition-temperature cuprate super-conductors. Nat Phys, 10(7):483–495, July 2014.

[43] Ralf Bulla, Theo A. Costi, and Thomas Pruschke. Numerical renormalization group method for quan-tum impurity systems. Rev. Mod. Phys., 80:395– 450, Apr 2008.

[44] V Yu Irkhin and MI Katsnelson. Theory of intermediate-valence semiconductors. Sov. Phys. JETP, 63:631, 1986.

[45] Shiro Sakai, Marcello Civelli, and Masatoshi Imada. Hidden fermionic excitation boosting high-temperature superconductivity in cuprates. Phys. Rev. Lett., 116:057003, Feb 2016.

[46] F. Verstraete, V. Murg, and J.I. Cirac. Matrix product states, projected entangled pair states, and variational renormalization group methods for quantum spin systems. Advances in Physics, 57(2): 143–224, 2008.

[47] V. Yu. Irkhin, A. A. Katanin, and M. I. Katsnel-son. Robustness of the van hove scenario for high-Tc superconductors. Phys. Rev. Lett., 89:076401, Jul 2002.